Various Rejuvenation Behaviors of Zr-Based Metallic Glass by Cryogenic Cycling Treatment with Different Casting Temperatures
- 133 Downloads
The rejuvenation behavior of an Zr50Cu40Al10 (at.%) metallic glass upon cryogenic cycling treatment has been investigated. At a high casting temperature, the microstructure of the glass is quite homogenous and thus, internal stress cannot be generated during cycling. Therefore, the glass cannot be rejuvenated by cryogenic cycling treatment. In the contrary, by lowering the casting temperature, nano-sized heterogeneity can be induced and subsequently generates the internal stress and rejuvenates the glass. Once the glass is rejuvenated, the more induced free volume can plasticize the glass with a higher plastic strain. These findings point out that the synthesis conditions can tailor the heterogeneity of the glass and subsequently affect the following rejuvenation behavior upon thermal treatment. It can also help understand the mechanisms of rejuvenation of metallic glass upon cryogenic cycling treatment.
KeywordsMetallic glass Rejuvenation Cryogenic cycling Casting temperature Heterogeneity
Bulk metallic glass
Deep cryogenic cycling treatment
Thermal treated with 30 cycles
Differential scanning calorimeter
Glass forming ability
High casting temperature
Low casting temperature
Transmission electron microscope
The bulk metallic glasses (BMGs) have attracted a lot of interests because of their superior mechanical properties such as high fracture strength and large elastic limit, which originates from their unique long-range disordered microstructures [1, 2, 3]. To suppress the nucleation and growth of crystalline phase during solidification, rapid quenching techniques are always required during the fabrication of BMGs [4, 5, 6]. The non-equilibrium solidification process makes BMGs possess higher configurational potential energy compared with their crystalline counterparts . Thus, during annealing, the microstructures of BMGs tend to change toward a lower energy state (relaxation), which makes them more like the crystalline counterparts . The so-called relaxation process of BMGs always degrades the properties of them, especially the mechanical properties, e.g., the embrittlement of BMGs after relaxation . Furthermore, the BMGs can even crystallize by supplying thermal or mechanical energy. Dudina et al. have investigated the crystallization behavior of Ti-Cu metallic glass under high-current density electrical pulses . They found that the crystallized microstructures of treated metallic glass vary with different pulse parameter and the crystalline phase can be as small as nano-size, which proves local melting and solidification during electrical pulse. In the contrary, the metastable BMGs can be also tailored to a higher energy state by both thermal and mechanical methods (rejuvenation), such as recovery annealing and severe plastic deformation [11, 12, 13]. Recently, Ketov et al. have found a novel deep cryogenic cycling treatment (DCT) to rejuvenate the BMGs, in which the samples are cooled and heated cyclically during room and cryogenic temperature (77 K) . The mechanism for this rejuvenation is considered to be the intrinsic heterogeneous structure of amorphous phase, which generates internal stress during cooling and heating. In this study, by using our original developed DCT instrument, the rejuvenation behavior of Zr50Cu40Al10 (at.%) during DCT have been investigated with cycling number of 30, denoted as DCT30. Two kinds of casting temperatures have been chosen by varying the heating current during copper mold casting, i.e., 9 A (high temperature) and 7 A (low temperature), denoted as HT and LT, respectively. The microstructures and mechanical properties of each sample are investigated in detail.
Master alloys were prepared by arc-melting high-purity Cu, Zr, and Al metal pieces in a Ti-gettered argon atmosphere in a water-cooled copper hearth. The BMG was fabricated by casting the master alloy into a copper mold to produce a 2-mm-diameter rod-shaped sample (As-cast sample). The original instrument to conduct DCT has been described in our previous study . By using this instrument, the samples can be cyclically cooled and heated between room temperature and 113 K.
The structures of the samples were examined by X-ray diffraction (XRD; Bruker D8 Advance) with Cu Kα radiation, and transmission electron microscopy (TEM, JEOL JEM-2100F) with an acceleration voltage of 200 kV. The glass transition temperature (Tg) and the onset crystalline temperature (Tx) were measured by differential scanning calorimeter (DSC) in argon at a heating rate of 20 K/min. The specific heat capacities were measured by comparing them with a sapphire standard sample. The density was measured using an Ar gas pycnometer (AccuPyc II 1340, Micromeritics Co. Ltd.). Compression tests were performed at a strain rate of 5 × 10−4 s−1 at room temperature using an Instron 5982 mechanical testing machine. Multiple compression tests using at least four samples each were conducted to confirm the reproducibility.
Results and Discussion
Rejuvenation Behavior of HT Samples
where ΔCp = Cp,s − Cp,r, and Cp,s and Cp,r are the specific heats of the sample and its relaxed state, respectively. In the present study, the relaxed state was obtained by annealing at 725 K (~ 1.05 Tg) for 2 min followed by a 20 K/min cooling. The specific heat curves of both samples and their relaxed state are plotted in Fig. 1d. Based on Eq. (1), ΔHrelax for As-cast and DCT30 was calculated to be ~ 12.6 J/g and 12.9 J/g, respectively. The similar ΔHrelax indicates that no rejuvenation occurs for the sample prepared at high casting temperature (HT samples).
A summary of thermal and mechanical data for the sample in this work
690 ± 5
780 ± 4
12.6 ± 0.2
12.6 ± 0.5
105 ± 5
2027 ± 15
1865 ± 22
2.3 ± 0.2
0.5 ± 0.2
688 ± 4
781 ± 5
12.5 ± 0.3
12.9 ± 0.3
114 ± 4
1983 ± 20
1873 ± 15
1.9 ± 0.1
0.2 ± 0.1
695 ± 5
781 ± 3
13.9 ± 0.5
10.7 ± 0.2
123 ± 5
1998 ± 18
1765 ± 18
4.3 ± 0.2
2.8 ± 0.2
697 ± 3
774 ± 5
14.2 ± 0.3
13.0 ± 0.3
107 ± 6
2049 ± 19
1640 ± 13
5.9 ± 0.3
4.3 ± 0.3
Our previous study on the rejuvenation behavior of Zr55Cu30Al10Ni5 (at.%) BMG upon DCT has shown that the intrinsic core-shell heterogeneity is the main reason of rejuvenation during cyclically cooling and heating. The different elastic modulus of core and shell generates internal stress upon DCT, which causes the evolution of core region with more induced free volume . Many researches have shown that the intrinsic heterogeneity of amorphous phase is related with the glass forming ability (GFA) of the alloy system [16, 17]. The BMG with a higher GFA possesses a more heterogeneous microstructure and subsequently causes rejuvenation upon DCT. However, for the sample in the present study, Zr50Cu40Al10 (at.%), the GFA is not as high as Zr55Cu30Al10Ni5 (at.%) [18, 19], thus, the more homogenous microstructure of Zr50Cu40Al10 cannot generate effective internal stress to rejuvenate the sample upon DCT.
Rejuvenation Behavior of LT Samples
where ΔHr is the crystallization enthalpy of the fully amorphous state and here we used the data of As-cast of HT sample (44.5 J/g). ΔHs of As-cast and DCT30 are 41.0 and 40.7 J/g, respectively. Thus, Vnc are calculated to be 7.8% and 8.5% for As-cast and DCT30, respectively. The similar Vnc before and after DCT indicates that the nano-clusters are stable and maintain no change upon DCT. In addition, the nano-clusters in LT samples may be B2-CuZr phase and thus ρnc is about 7.45 g/cm3 [22, 23]. By using the data shown above with Eqs. (2) and (3), x of As-cast and DCT30 are calculated to be 1.30% and 2.06%, respectively, which suggests that more free volume has been induced for LT samples upon DCT and the BMGs are rejuvenated. It agrees well with the results from thermal analysis.
The homogenous amorphous structure in HT samples cannot generate internal stress to rejuvenate themselves. In the contrary, the LT samples which have the same composition and cooling rate (same size of sample) can be rejuvenated upon DCT. This difference should originate from the microstructure. Figure 4b, c shows the TEM images of As-cast and DCT30 which are cast at low temperature, respectively. Apparently, very fine nano-sized clusters can be observed for both samples, which is different from the structure of HT sample shown in Fig. 2a, b.
where Δα is the thermal expansion coefficient differences between the amorphous and crystalline phases, ΔT is the temperature change, Ec and Ea are the elastic modulus for the crystalline and amorphous phases, respectively, and νc and νa are the Poisson’s ratio for crystalline and amorphous phases, respectively. Previous study has shown that the nano-clusters may be B2-CuZr phase . The thermal expansion coefficients for the amorphous and crystalline phases have been reported to be ~ 1.3 × 10−5 K−1 and 1.14 × 10−5 K−1, respectively , Ec and Ea have been reported to be ~ 77 and 123 GPa, respectively , and νc and νa have been reported to be ~ 0.385 and 0.383, respectively [28, 29]. ΔT was ~ 180 K (293 K to 113 K). Thus, by using Eq. (5), σα is calculated to be ~ 34 MPa, which causes local atomic rearrangement and also helps to rejuvenate the amorphous phase.
As the intrinsic heterogeneity of BMGS can affect the rejuvenation behavior of BMGs upon following thermal treatment, the reason why different casting temperatures can tailor the microstructures should be clarified. Zhu et al. have also found that the casting temperature can tailor the structure from fully amorphous state (at high casting temperature) to composite structure (at low casting temperature) . When the metallic liquid is quenched from high temperature, the element in the liquid can be fully mixed and makes the liquid more homogenous. Thus, fully amorphous phase can be obtained. However, if the casting temperature is low, the element segregation can occur in very local area among the liquid, which are retained during the solidification. This segregation is considered to be the nuclei for the nano-clusters in LT samples. Furthermore, if the casting temperature is very low, we cannot produce amorphous samples even with high cooling rate. Therefore, varying the casting temperature can induce nano-sized heterogeneity in the amorphous matrix, which generates internal stress and rejuvenation during DCT.
In the present study, the rejuvenation behaviors of Zr50Cu40Al10 (at.%) BMGs upon DCT have been investigated. At high casting temperature, for the fully mixing of elements, fully amorphous phase with quite homogeneous structure can be fabricated after quenching. No rejuvenation occurs for these samples because of the lack of internal stress during cyclically cooling and heating. In the contrary, at low casting temperature, for the element segregation, nano-cluster dispersed amorphous structure can be observed, which generates high internal stress and causes the rejuvenation of samples upon DCT. The rejuvenated sample with more free volume shows better plasticity than As-cast ones. These findings provide a novel method to tailor the microstructure of as-cast BMG samples, which affects both the mechanical properties and rejuvenation behavior during the following DCT treatment.
W. Guo is grateful for the financial support of start-up fund (No. 3004110125) from Huazhong University of Science and Technology
This work was supported by Huazhong University of Science and Technology under Grant [number 3004110125].
Availability of Data and Materials
The datasets used and/or analyzed during the current study are available from the corresponding author on reasonable request.
Conceptualization, WG and JS; methodology, WG; validation, WG, JS; formal analysis, WG; investigation, SW.; resources, JS and SW; writing—original draft preparation, WG; writing—review and editing, JS; supervision, JS and SW; project administration, WG; funding acquisition, WG and SW. All authors read and approved the final manuscript.
The authors declare that they have no competing interests.
Springer Nature remains neutral with regard to jurisdictional claims in published maps and institutional affiliations.
Open AccessThis article is distributed under the terms of the Creative Commons Attribution 4.0 International License (http://creativecommons.org/licenses/by/4.0/), which permits unrestricted use, distribution, and reproduction in any medium, provided you give appropriate credit to the original author(s) and the source, provide a link to the Creative Commons license, and indicate if changes were made.